Cellular solid structures with unbounded thermal expansion. Roderic Lakes. Journal of Materials Science Letters, 15, (1996).


 Drusilla Bruce
 1 years ago
 Views:
Transcription
1 1 Cellular solid structures with unbounded thermal expansion Roderic Lakes Journal of Materials Science Letters, 15, (1996). Abstract Material microstructures are presented which can exhibit coefficients of thermal expansion larger than that of either constituent. Thermal expansion of materials is of considerable practical interest since materials in service may experience a considerable range of operating temperature. Materials with microstructure, including composites, honeycombs, and foams (which are composites with one void phase) are finding increasing application for many purposes. It is therefore of interest to explore the range of thermal expansion coefficient attainable in materials with microstructure. The constitutive equation for a linear isotropic thermoelastic continuum is [1]: ε ij = 1 + ν E σ ij  [ ν E σ ii  α T]δ ij, (1) in which ε ij is strain, σ ij is stress, ν is Poisson's ratio, E is Young's modulus, α is the thermal expansion coefficient, δ ij is Kronecker's delta, and the usual index notation is used. Thermal expansion of crystalline solids is considered to arise from the anharmonicity of the interatomic potential. Thermal expansion coefficients for solids are on the order of 3 x 106 / C for ceramics, 105 / C for metals, and 104 / C for polymers [2]; many specific values are given in reference [3]. Thermal expansion of foams was discussed briefly by Gibson and Ashby [2] who pointed out that for a foam viewed as a framework (of homogeneous ribs), the thermal expansion coefficient is the same as the solid from which it is made. An exception is a closed cell foam of very small solid volume fraction, for which thermal expansion is enhanced by the expansion of the gas within the cells [2]. An upper bound for this effect can be estimated as follows. If the foam is very compliant, expansion of the gas occurs at approximately constant pressure. Considering the ideal gas law PV = nrt, the expansion of such a compliant foam at room temperature (T = 300 K) can be no more than α = 1.1 x 103 / C, greater than that of a solid polymer. For arbitrary twophase composite materials, bounds have been developed for the thermal expansion coefficient α of the composite in terms of that of each constituent [4,5]; the upper bound is a rule of mixtures. In deriving these bounds it was assumed that there are only two phases, and there is no empty space in the composite. In the present work, it is shown that if one relaxes the
2 2 assumption of no empty space, it is possible to generate cellular microstructures which exhibit a thermal expansion coefficient much larger than that of either constituent. Consider a cellular solid consisting of bilayer ribs. The rib element in the cellular solid consists of a laminate of two layers of differing thermal expansion coefficient α. The layers have Young's moduli E 1 and E 2, Poisson's ratio ν 1 and ν 2 ; thermal expansion coefficient α 1 and α 2 ; and thicknesses h 1 and h 2. The curvature κ (the inverse of the radius of curvature ρ) of a thin bilayer elastic beam is given in terms of the temperature change T by Timoshenko [6], neglecting end effects [7]. The curvature may be written κ = 6(α 2  α 1 ) T (1 + h 1 h 2 ) 2 (h 1 + h 2 ) 1 3((1 + h 1 h ) 2 ) + (1 + h 1 E 1 2 h 2 E ) (( h 1 2 h ) 2 + h 2E 2 2 h 1 E ) 1. (2) The curvature can be made arbitrarily large by making the strip thickness h small. The ratio of Young's moduli has little effect on the curvature [6]. We determine the thermal expansion coefficient of cellular solids with twolayer rib elements. Consider first the deformations and strains caused by rib curvature due to strain. The transverse displacement δ at the midpoint of an initially straight rib of length l is [6] δ = κl2 8. (3) Cellular solids which exhibit global thermal expansion due to such transverse rib displacements must have an unusual connectivity, such as that shown in Fig. 1. It is easier to make use of longitudinal displacement of rib elements as determined as follows. Referring to Fig. 2, consider now a curved rib element of arc length l arc, radius of curvature r, and included angle θ, in radians. The rib length is given by l = l arc 2 θ sin θ 2. (4) The strain of a unit cell due to end to end length changes in the rib is ε = dl l. (5) The effect of a curvature increment dκ due to bending is ε = [ 1 2 ctn θ 21 θ ] l arcdκ. (6)
3 3 Eq. 2 gives the curvature of a straight rib, or the increment in curvature of an initially curved rib. Eq. 6 shows that there must be some initial curvature or no finite length change occurs. Cellular solids which expand due to longitudinal displacement by bending of ribs with initial curvature are shown in Fig. 3. The thermal expansion coefficient of the cellular solid structure is α = ε/ T (at constant stress, see Eq. 1), so α = l arc (h 1 + h 2 ) 6(α 2  α 1 )(1 + h 1 h 2 ) 2 3((1 + h 1 h ) 2 ) + (1 + h 1 E 1 2 h 2 E ) (( h 1 2 h ) 2 + h 2E 2 2 h 1 E ) 1 [ 1 2 ctn θ 21 θ ] (7) The ratio of rib arc length to rib total thickness can be made arbitrarily large, by making the ribs very slender. The initial curvature of the ribs, as quantified by the included angle θ, should also be made large in order to maximize the magnitude of α given by Eq. 7 (Fig. 4). The thermal expansion coefficient of the cellular solid structure is therefore unbounded. It can be made much larger in magnitude than the thermal expansion coefficient of either solid constituent. The sign of the thermal expansion coefficient of the cellular solid is governed by the placement of the constituents within each rib. Referring to Fig. 3, if the constituent with the higher thermal expansion coefficient is on its concave side, an increase in temperature will cause the rib to straighten, giving rise to a positive thermal expansion coefficient for the cellular solid. Conversely, if the constituent with the higher thermal expansion coefficient is on its convex side, an increase in temperature will cause the rib to curve more and become shorter, giving rise to a negative thermal expansion coefficient for the cellular solid. The structure shown in Fig. 3 has two dimensional cubic symmetry giving rise to anisotropic elasticity but isotropic thermal expansion. Hexagonal structures which are elastically isotropic in plane are also possible. The examples presented are twodimensional honeycombs. They could be produced by a coextrusion process, by progressive lamination, or by lithography. One may also envisage threedimensional cellular solids, or foams, containing bilayer ribs, which may be sintered together. Materials based on polymer bilayers can deliver higher thermal expansion than those based on metallic bilayers. These structures provide a further illustration of the importance of void space in determining physical properties. Inclusion of void space permits one to substantially exceed bounds for thermal expansion developed under the assumption of no void space. Control of the shape of void space has led to materials with a negative Poisson's ratio [8] and lightweight hierarchical materials with high ratios of strength to weight [9]. More developments in materials with unusual or extreme properties are anticipated.
4 4 To conclude, arbitrarily high values of thermal expansion can be attained by preparing cellular solids with ribs consisting of a bilayer containing materials of two different expansion coefficients. References 1 I. S. Sokolnikoff, Mathematical theory of elasticity, (Krieger, Malabar, FL, 2nd ed., 1983). 2 L. J. Gibson and M.F. Ashby, Cellular Solids (Pergamon press, Oxford, 1987). 3 Staff, "Comparison of materials; coefficient of thermal expansion", Materials Engineering 103 (1986) J. L. Cribb, "Shrinkage and thermal expansion of a twophase material", Nature, 220 (1963) S. Torquato, "Bounds on the thermoelastic properties of suspensions of spheres", J. Appl. Phys. 67, (1990), S. P. Timoshenko, "Analysis of bimetal thermostats", J. Optical Soc. America, 11 (1925) E. Suhir, "Stresses in bimetal thermostats", J. Appl. Mech., 53 (1986) R.S. Lakes, "Foam structures with a negative Poisson's ratio", Science, 235 (1987) R.S. Lakes, "Materials with structural hierarchy", Nature, 361, (1993)
5 5 Figures 1 Cellular solid which undergoes thermal expansion via lateral bending displacement of ribs. 2 Rib element geometry with initial curvature. l arc = θ l l/2 θ r θ /2 r
6 6 3 Cellular solid with curved ribs. It undergoes thermal expansion via longitudinal bending displacement of ribs.
7 7 4 Normalized thermal expansion and rib aspect ratio l arc h α α 2  α 1 of cellular solid vs. rib curve angle θ (in radians) for h 1 = h 2 = h and E 1 = E 2.
Piezoelectric composite lattices with high sensitivity
Piezoelectric composite lattices with high sensitivity Roderic Lakes Department of Engineering Physics, Engineering Mechanics Program, Department of Materials Science, Rheology Research Center, University
More informationProperties of a chiral honeycomb with a Poisson's ratio 1
Properties of a chiral honeycomb with a Poisson's ratio 1 D. Prall, R. S. Lakes Int. J. of Mechanical Sciences, 39, 305314, (1996). Abstract A theoretical and experimental investigation is conducted
More informationThreedimensional stiff cellular structures with negative Poisson's ratio
! Threedimensional stiff cellular structures with negative Poisson's ratio Dong Li a, Jie Ma a, Liang Dong b and Roderic S. Lakes c a College of Sciences, Northeastern University, Shenyang 110819, PR
More informationAnalysis of high loss viscoelastic composites
Analysis of high loss viscoelastic composites by C. P. Chen, Ph.D. and R. S. Lakes, Ph.D. Department of Engineering Physics Engineering Mechanics Program; Biomedical Engineering Department Materials Science
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationLecture 4 Honeycombs Notes, 3.054
HoneycombsInplane behavior Lecture 4 Honeycombs Notes, 3.054 Prismatic cells Polymer, metal, ceramic honeycombs widely available Used for sandwich structure cores, energy absorption, carriers for catalysts
More informationSTRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLASFIR
UNITED STATES DEPARTMENT OF AGRICULTURE. FOREST SERVICE  FOREST PRODUCTS LABORATORY  MADISON, WIS. STRESSES WITHIN CURVED LAMINATED BEAMS OF DOUGLASFIR NOVEMBER 1963 FPL020 STRESSES WITHIN CURVED LAMINATED
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationA short review of continuum mechanics
A short review of continuum mechanics Professor Anette M. Karlsson, Department of Mechanical ngineering, UD September, 006 This is a short and arbitrary review of continuum mechanics. Most of this material
More informationCurvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment. P. Krulevitch G. C. Johnson
UCRLJC30440 PREPRINT Curvature of a Cantilever Beam Subjected to an EquiBiaxial Bending Moment P. Krulevitch G. C. Johnson This paper was prepared for submittal to the Materials Research Society Spring
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationChoi, J. B. and Lakes, R. S., "Nonlinear properties of polymer cellular materials with a negative Poisson's. ratio",
1 Choi, J. B. and Lakes, R. S., "Nonlinear properties of polymer cellular materials with a negative Poisson's ratio", J. Materials Science, 27, 46784684 (1992). Cover issue. ABSTRACT Negative Poisson's
More informationELECTROMECHANICAL RESPONSE OF PIEZOELECTRIC FOAMS
18 TH INTRNATIONAL CONFRNC ON COMPOSIT MATRIALS LCTROMCHANICAL RSPONS OF PIZOLCTRIC FOAMS K.S. Challagulla 1 *, T.A. Venkatesh 1 School of ngineering, Laurentian University, Sudbury, Canada, Department
More informationLaminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
United States Department of Agriculture Forest Service Forest Products Laboratory Research Paper FPL 375 June 1980 Laminated Beams of Isotropic or Orthotropic Materials Subjected to Temperature Change
More informationMacroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs
Macroscopic Elastic Constitutive Relationship of CastinPlace HollowCore Slabs JingZhong Xie 1 Abstract: The macroscopic Poisson ratio and elastic moduli of the castinplace hollowcore slab are researched
More informationADVANCES IN NEGATIVE POISSON'S RATIO MATERIALS. Roderic Lakes adapted from Advanced Materials, 5, , (1993). Diagrams at bottom.
1 ADVANCES IN NEGATIVE POISSON'S RATIO MATERIALS Roderic Lakes adapted from Advanced Materials, 5, 293296, (1993). Diagrams at bottom. 1. Introduction Poisson's ratio of a solid is defined as the lateral
More informationLarge Thermal Deflections of a Simple Supported Beam with TemperatureDependent Physical Properties
Large Thermal Deflections of a Simple Supported Beam with TemperatureDependent Physical Properties DR. ŞEREF DOĞUŞCAN AKBAŞ Civil Engineer, Şehit Muhtar Mah. Öğüt Sok. No:2/37, 34435 Beyoğlu Istanbul,
More informationENGN 2340 Final Project Report. Optimization of Mechanical Isotropy of Soft Network Material
ENGN 2340 Final Project Report Optimization of Mechanical Isotropy of Soft Network Material Enrui Zhang 12/15/2017 1. Introduction of the Problem This project deals with the stressstrain response of a
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationMeasurement of deformation. Measurement of elastic force. Constitutive law. Finite element method
Deformable Bodies Deformation x p(x) Given a rest shape x and its deformed configuration p(x), how large is the internal restoring force f(p)? To answer this question, we need a way to measure deformation
More informationStresses in Curved Beam
Stresses in Curved Beam Consider a curved beam subjected to bending moment M b as shown in the figure. The distribution of stress in curved flexural member is determined by using the following assumptions:
More informationComposite materials: mechanical properties
Composite materials: mechanical properties A computational lattice model describing scale effects @ nanoscale Luciano Colombo In collaboration with: Pier Luca Palla and Stefano Giordano Department of
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More information3D Elasticity Theory
3D lasticity Theory Many structural analysis problems are analysed using the theory of elasticity in which Hooke s law is used to enforce proportionality between stress and strain at any deformation level.
More informationStability of Cosserat solids: size effects, ellipticity and waves
Stability of Cosserat solids: size effects, ellipticity and waves Roderic S. Lakes Department of Engineering Physics, Engineering Mechanics Program Department of Materials Science, Rheology Research Center,
More informationMechanics of Irregular Honeycomb Structures
Mechanics of Irregular Honeycomb Structures S. Adhikari 1, T. Mukhopadhyay 1 Chair of Aerospace Engineering, College of Engineering, Swansea University, Singleton Park, Swansea SA2 8PP, UK Sixth International
More informationEE C247B / ME C218 INTRODUCTION TO MEMS DESIGN SPRING 2014 C. Nguyen PROBLEM SET #4
Issued: Wednesday, Mar. 5, 2014 PROBLEM SET #4 Due (at 9 a.m.): Tuesday Mar. 18, 2014, in the EE C247B HW box near 125 Cory. 1. Suppose you would like to fabricate the suspended cross beam structure below
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationMechanics PhD Preliminary Spring 2017
Mechanics PhD Preliminary Spring 2017 1. (10 points) Consider a body Ω that is assembled by gluing together two separate bodies along a flat interface. The normal vector to the interface is given by n
More informationThe fracture toughness of planar lattices: imperfection sensitivity
1 2 The fracture toughness of planar lattices: imperfection sensitivity 3 Naomi E.R. Romijn, Norman A. Fleck 4 5 Cambridge University Engineering Department, Trumpington Street, Cambridge CB2 1PZ, UK 6
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More information16.21 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive Equations
6.2 Techniques of Structural Analysis and Design Spring 2003 Unit #5  Constitutive quations Constitutive quations For elastic materials: If the relation is linear: Û σ ij = σ ij (ɛ) = ρ () ɛ ij σ ij =
More informationFundamentals of Linear Elasticity
Fundamentals of Linear Elasticity Introductory Course on Multiphysics Modelling TOMASZ G. ZIELIŃSKI bluebox.ippt.pan.pl/ tzielins/ Institute of Fundamental Technological Research of the Polish Academy
More informationPROPAGATION OF CURVED CRACKS IN HOMOGENEOUS AND GRADED MATERIALS
PROPAGATION OF CURVED CRACKS IN HOMOGENEOUS AND GRADED MATERIALS Abstract Matthew T. Tilbrook, Robert J. Moon and Mark Hoffman School of Materials Science and Engineering University of New South Wales,
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationLecture 7, Foams, 3.054
Lecture 7, Foams, 3.054 Opencell foams StressStrain curve: deformation and failure mechanisms Compression  3 regimes  linear elastic  bending  stress plateau  cell collapse by buckling yielding
More informationReduced warp in torsion of reticulated foam due to Cosserat elasticity: experiment
Reduced warp in torsion of reticulated foam due to Cosserat elasticity: experiment Roderic S. Lakes May 25, 2016 Department of Engineering Physics, Department of Materials Science University of Wisconsin,
More informationStrain Gages. Approximate Elastic Constants (from University Physics, Sears Zemansky, and Young, Reading, MA, Shear Modulus, (S) N/m 2
When you bend a piece of metal, the Strain Gages Approximate Elastic Constants (from University Physics, Sears Zemansky, and Young, Reading, MA, 1979 Material Young's Modulus, (E) 10 11 N/m 2 Shear Modulus,
More informationThe Rotating Inhomogeneous Elastic Cylinders of. VariableThickness and Density
Applied Mathematics & Information Sciences 23 2008, 237 257 An International Journal c 2008 Dixie W Publishing Corporation, U. S. A. The Rotating Inhomogeneous Elastic Cylinders of VariableThickness and
More informationCHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles
CHEMC2410: Materials Science from Microstructures to Properties Composites: basic principles Mark Hughes 14 th March 2017 Today s learning outcomes To understand the role of reinforcement, matrix and
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationA Note on Suhir s Solution of Thermal Stresses for a DieSubstrate Assembly
M. Y. Tsai email: mytsai@mail.cgu.edu.tw C. H. Hsu C. N. Han Department of Mechanical Engineering, Chang Gung University, KweiShan, TaoYuan, Taiwan 333, ROC A Note on Suhir s Solution of Thermal Stresses
More informationChapter 2: Elasticity
OHP 1 Mechanical Properties of Materials Chapter 2: lasticity Prof. Wenjea J. Tseng ( 曾文甲 ) Department of Materials ngineering National Chung Hsing University wenjea@dragon.nchu.edu.tw Reference: W.F.
More informationSupplementary Figures
Supplementary Figures 8 6 Energy (ev 4 2 2 4 Γ M K Γ Supplementary Figure : Energy bands of antimonene along a highsymmetry path in the Brillouin zone, including spinorbit coupling effects. Empty circles
More informationForced Response of Plate with Viscoelastic Auxetic Dampers
Vibrations in Physical Systems 2018, 29, 2018003 (1 of 9) Abstract Forced Response of Plate with Viscoelastic Auxetic Dampers Tomasz STREK Poznan University of Technology, Institute of Applied Mechanics
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationPrediction of Elastic Constants on 3D Fourdirectional Braided
Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Prediction of Elastic Constants on 3D Fourdirectional Braided Composites Liang Dao Zhou 1,2,* and Zhuo Zhuang 1 1 School of Aerospace,
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationTHE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF ORIENTED STRANDBOARD: A FINITE ELEMENT SIMULATION
Proceedings of McMat5: 5 Joint ASME/ASCE/SES Conference on Mechanics and Materials June 13, 5, Baton Rouge, Louisiana, USA 255 THE INFLUENCE OF INPLANE DENSITY VARIATION ON ENGINEERING PROPERTIES OF
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationBENCHMARK LINEAR FINITE ELEMENT ANALYSIS OF LATERALLY LOADED SINGLE PILE USING OPENSEES & COMPARISON WITH ANALYTICAL SOLUTION
BENCHMARK LINEAR FINITE ELEMENT ANALYSIS OF LATERALLY LOADED SINGLE PILE USING OPENSEES & COMPARISON WITH ANALYTICAL SOLUTION Ahmed Elgamal and Jinchi Lu October 07 Introduction In this study: I) The response
More informationEffect of Growth Direction on Twin Formation in GaAs Crystals Grown by the Vertical Gradient Freeze Method
Effect of Growth Direction on Twin Formation in GaAs Crystals Grown by the Vertical Gradient Freeze Method A.N. Gulluoglu 1,C.T.Tsai 2 Abstract: Twins in growing crystals are due to excessive thermal stresses
More informationCharacterisation and Modelling of a MeltExtruded LDPE Closed Cell Foam
Characterisation and Modelling of a MeltExtruded LDPE Closed Cell Foam Qusai Hatem Jebur 1,a, Philip Harrrison 1,b, Zaoyang Guo,c, Gerlind Schubert 1,d & Vincent Navez 3,e 1 School of Engineering, University
More informationThe aims of this experiment were to obtain values for Young s modulus and Poisson s ratio for
The Cornu Method Nikki Truss 09369481 Abstract: The aims of this experiment were to obtain values for Young s modulus and Poisson s ratio for Perspex using the Cornu Method. A value of was found for Young
More informationExample 3.7 Consider the undeformed configuration of a solid as shown in Figure 3.60.
162 3. The linear 3D elasticity mathematical model The 3D elasticity model is of great importance, since it is our highest order hierarchical model assuming linear elastic behavior. Therefore, it provides
More informationKeywords: Reentrant; cellular solid; Negative Poisson s ratio; Voronoi; Energy absorption; Compression
Negative Poisson's ratio in 2D Voronoi cellular solids by biaxial compression: a numerical study Preprint: Li, D. Dong, L., Yin, J. and Lakes, R. S., "Negative Poisson's ratio in 2D Voronoi cellular solids
More informationUSING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE
Volume II: Fatigue, Fracture and Ceramic Matrix Composites USING A HOMOGENIZATION PROCEDURE FOR PREDICTION OF MATERIAL PROPERTIES AND THE IMPACT RESPONSE OF UNIDIRECTIONAL COMPOSITE A. D. Resnyansky and
More informationLecture 7: The Beam Element Equations.
4.1 Beam Stiffness. A Beam: A long slender structural component generally subjected to transverse loading that produces significant bending effects as opposed to twisting or axial effects. MECH 40: Finite
More informationTheories of Straight Beams
EVPM3ed02 2016/6/10 7:20 page 71 #25 This is a part of the revised chapter in the new edition of the tetbook Energy Principles and Variational Methods in pplied Mechanics, which will appear in 2017. These
More informationSupplementary figures
Supplementary figures Supplementary figure 1: The fang model (longitudinal section) used for the stiffness analysis. The base of the fang is considered fixed (i.e. zero displacement constraint) and the
More informationPEAT SEISMOLOGY Lecture 2: Continuum mechanics
PEAT8002  SEISMOLOGY Lecture 2: Continuum mechanics Nick Rawlinson Research School of Earth Sciences Australian National University Strain Strain is the formal description of the change in shape of a
More information4. BEAMS: CURVED, COMPOSITE, UNSYMMETRICAL
4. BEMS: CURVED, COMPOSITE, UNSYMMETRICL Discussions of beams in bending are usually limited to beams with at least one longitudinal plane of symmetry with the load applied in the plane of symmetry or
More informationBasic Equations of Elasticity
A Basic Equations of Elasticity A.1 STRESS The state of stress at any point in a loaded bo is defined completely in terms of the nine components of stress: σ xx,σ yy,σ zz,σ xy,σ yx,σ yz,σ zy,σ zx,andσ
More informationElasticity in two dimensions 1
Elasticity in two dimensions 1 Elasticity in two dimensions Chapters 3 and 4 of Mechanics of the Cell, as well as its Appendix D, contain selected results for the elastic behavior of materials in two and
More informationFrequently Asked Questions
Frequently Asked Questions Why do we have to make the assumption that plane sections plane? How about bars with nonaxis symmetric cross section? The formulae derived look very similar to beam and axial
More informationRegular, low density cellular structures  rapid prototyping, numerical simulation, mechanical testing
Mat. Res. Soc. Symp. Proc. Vol. 823 2004 Materials Research Society W8.8.1 Regular, low density cellular structures  rapid prototyping, numerical simulation, mechanical testing J. Stampfl 1, M.M. Seyr
More informationThe New Boundary Condition Effect on The Free Vibration Analysis of Microbeams Based on The Modified Couple Stress Theory
International Research Journal of Applied and Basic Sciences 2015 Available online at www.irjabs.com ISSN 2251838X / Vol, 9 (3): 274279 Science Explorer Publications The New Boundary Condition Effect
More informationDYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD
ECCM66 TH EUROPEAN CONFERENCE ON COMPOSITE MATERIALS, Seville, Spain, 6 June 4 DYNAMIC RESPONSE OF SYNTACTIC FOAM CORE SANDWICH USING A MULTIPLE SCALES BASED ASYMPTOTIC METHOD K. V. Nagendra Gopal a*,
More informationMICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING
MICROMECHANICAL ANALYSIS OF FRP COMPOSITES SUBJECTED TO LONGITUDINAL LOADING N. Krishna Vihari 1, P. Phani Prasanthi 1, V. Bala Krishna Murthy 2* and A. Srihari Prasad 3 1 Mech. Engg. Dept., P. V. P. Siddhartha
More informationMASSACHUSETTS INSTITUTE OF TECHNOLOGY DEPARTMENT OF MATERIALS SCIENCE AND ENGINEERING CAMBRIDGE, MASSACHUSETTS 02139
MASSACHUSTTS INSTITUT OF TCHNOLOGY DPARTMNT OF MATRIALS SCINC AND NGINRING CAMBRIDG, MASSACHUSTTS 0239 322 MCHANICAL PROPRTIS OF MATRIALS PROBLM ST 4 SOLUTIONS Consider a 500 nm thick aluminum ilm on a
More informationConsider an elastic spring as shown in the Fig.2.4. When the spring is slowly
.3 Strain Energy Consider an elastic spring as shown in the Fig..4. When the spring is slowly pulled, it deflects by a small amount u 1. When the load is removed from the spring, it goes back to the original
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationStrong Cosserat elastic effects in a unidirectional composite
Strong Cosserat elastic effects in a unidirectional composite Zach Rueger and Roderic S. Lakes September 20, 2018 Department of Engineering Physics, Department of Materials Science University of Wisconsin,
More informationCHAPTER OBJECTIVES Use various methods to determine the deflection and slope at specific pts on beams and shafts: 2. Discontinuity functions
1. Deflections of Beams and Shafts CHAPTER OBJECTIVES Use various methods to determine the deflection and slope at specific pts on beams and shafts: 1. Integration method. Discontinuity functions 3. Method
More informationTHE TOPOLOGICAL DESIGN OF MATERIALS WITH SPECIFIED THERMAL EXPANSION USING A LEVEL SETBASED PARAMETERIZATION METHOD
11th. World Congress on Computational Mechanics (WCCM XI) 5th. European Conference on Computational Mechanics (ECCM V) 6th. European Conference on Computational Fluid Dynamics (ECFD VI) July 2025, 2014,
More informationViscoelastic Properties of Foamed Thermoplastic Vulcanizates and their Dependence on Void Fraction
Viscoelastic Properties of Foamed Thermoplastic Vulcaniates and their Dependence on Void Fraction Viscoelastic Properties of Foamed Thermoplastic Vulcaniates and their Dependence on Void Fraction Junhong
More informationMODIFIED HYPERBOLIC SHEAR DEFORMATION THEORY FOR STATIC FLEXURE ANALYSIS OF THICK ISOTROPIC BEAM
MODIFIED HYPERBOLIC SHEAR DEFORMATION THEORY FOR STATIC FLEXURE ANALYSIS OF THICK ISOTROPIC BEAM S. Jasotharan * and I.R.A. Weerasekera University of Moratuwa, Moratuwa, Sri Lanka * EMail: jasos91@hotmail.com,
More informationElements of Continuum Elasticity. David M. Parks Mechanics and Materials II February 25, 2004
Elements of Continuum Elasticity David M. Parks Mechanics and Materials II 2.002 February 25, 2004 Solid Mechanics in 3 Dimensions: stress/equilibrium, strain/displacement, and intro to linear elastic
More informationCHAPTER 5. Beam Theory
CHPTER 5. Beam Theory SangJoon Shin School of Mechanical and erospace Engineering Seoul National University ctive eroelasticity and Rotorcraft Lab. 5. The EulerBernoulli assumptions One of its dimensions
More informationCHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement
CHEME2200: Polymer blends and composites Fibre architecture and principles of reinforcement Mark Hughes 19 th September 2016 Outline Fibre architecture Volume fraction and the rule of mixtures Principle
More informationLecture 8. Stress Strain in Multidimension
Lecture 8. Stress Strain in Multidimension Module. General Field Equations General Field Equations [] Equilibrium Equations in Elastic bodies xx x y z yx zx f x 0, etc [2] Kinematics xx u x x,etc. [3]
More informationOn the viscoelastic properties of opencell polyurethane foams in uniaxial compression
Author manuscript, published in "6th International Congress of the Croatian Society of Mechanics, Dubrovnik : Croatia (2009)" On the viscoelastic properties of opencell polyurethane foams in uniaxial
More informationStrain Gages. Approximate Elastic Constants (from University Physics, Sears Zemansky, and Young, Reading, MA, 1979
Material Strain Gages Approximate Elastic Constants (from University Physics, Sears Zemansky, and Young, Reading, MA, 1979 Young's Modulus, Y Shear Modulus, S Bulk Modulus, B Poisson's Ratio 10 11 N/m
More information3 2 6 Solve the initial value problem u ( t) 3. a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1
Math Problem a If A has eigenvalues λ =, λ = 1 and corresponding eigenvectors 1 3 6 Solve the initial value problem u ( t) = Au( t) with u (0) =. 3 1 u 1 =, u 1 3 = b True or false and why 1. if A is
More informationFOAM TOPOLOGY BENDING VERSUS STRETCHING DOMINATED ARCHITECTURES
Acta mater. 49 (001) 1035 1040 www.elsevier.com/locate/actamat FOAM TOPOLOGY BENDING VERSUS STRETCHING DOMINATED ARCHITECTURES V. S. DESHPANDE, M. F. ASHBY and N. A. FLECK Cambridge University, Department
More informationINFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK BETWEEN THE TWO LAYERS
Djoković, J. M., et.al.: Influence of Temperature on Behavior of the Interfacial THERMAL SCIENCE: Year 010, Vol. 14, Suppl., pp. S59S68 S59 INFLUENCE OF TEMPERATURE ON BEHAVIOR OF THE INTERFACIAL CRACK
More informationMechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach
Mechanical and Thermal Properties of Coir Fiber Reinforced Epoxy Composites Using a Micromechanical Approach Sandhyarani Biswas Department of Mechanical Engineering, N.I.T Rourkela, INDIA Abstract: Nowadays,
More informationInternational Journal of Scientific & Engineering Research Volume 8, Issue 12, December2017 ISSN
362 Study of the Effects of Random Inclusions in Composite Construction with Isotropic Negative Poisson s Ratio [Kundan Singh Deshwal1, a and Dr. Satyendra Singh2, b] 1 Assistant Professor, Department
More informationASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS
ASSESSMENT OF MIXED UNIFORM BOUNDARY CONDITIONS FOR PREDICTING THE MACROSCOPIC MECHANICAL BEHAVIOR OF COMPOSITE MATERIALS Dieter H. Pahr and Helmut J. Böhm Institute of Lightweight Design and Structural
More informationModule 7: Micromechanics Lecture 25: Strength of Materials Approach. Introduction. The Lecture Contains. Effective Transverse Modulus
Introduction In the previous lecture we have introduced the concept of Representative Volume Element or Unit Cell. This is the basic building block in a micromechanical study. Further, we explained the
More informationInternational Journal of Pure and Applied Sciences and Technology
Int. J. Pure Appl. Sci. Technol., 3() (0), pp. 739 International Journal of Pure and Applied Sciences and Technology ISSN 9607 Available online at www.ijopaasat.in Research Paper Reflection of Quasi
More informationViscoelastic Damping Characteristics of IndiumTin/SiC Particulate Composites
Viscoelastic Damping Characteristics of IndiumTin/SiC Particulate Composites HyungJoo Kim, Colby C. Swan Ctr. for ComputerAided Design, Univ. of Iowa Roderic Lakes Engineering Physics, Univ. of Wisconsin
More information